California Test 202
STATE OF CALIFORNIA—BUSINESS, TRANSPORTATION AND HOUSING AGENCY November 2011
DEPARTMENT OF TRANSPORTATION
DIVISION OF ENGINEERING SERVICES
5900 Folsom Boulevard
Sacramento, California 95819-4612
METHOD OF TEST FOR SIEVE ANALYSIS OF
FINE AND COARSE AGGREGATES
This method, which includes modifications of AASHTO Designations T 11, T 27, T 30, and T 37,
specifies the procedures for determining the particle-size distribution of fine and coarse
Special procedures for testing aggregate from extracted bituminous mixtures, supplemental fine
aggregate, glass spheres, and granular quicklime are included in Appendices A, B, C, and D,
respectively. A procedure for expediting testing and providing an approximate particle-size
distribution for processed fine aggregate is included in Appendix E.
California Test 201- Soil and Aggregate Sample Preparation
AASHTO M 92 - Standard Specification for Wire-Cloth Sieves for Testing Purposes
AASHTO T 11 - Test for Materials Finer Than 75-μm (No. 200) Sieve in Mineral Aggregates
AASHTO T 27 - Test for Sieve Analysis of Fine and Coarse Aggregates
AASHTO T 30 - Test for Mechanical Analysis of Extracted Aggregate
AASHTO T 37 - Test for Sieve Analysis of Mineral Filler for Hot Mix Asphalt (HMA)
1. Balance: A balance or scale reading to 1 g for samples weighing less than
approximately 1,000 g. For samples weighing more than 1,000 g the balance or
scale should read to 0.2 % of the test sample’s mass.
2. Sieves: Woven-wire cloth sieves of 3 in., 2 ½ in., 2 in., 1 ½ in., 1 in., ¾ in., ½ in.,
3/8 in., ¼ in., No. 4, No. 8, No. 16, No. 30, No. 50, No. 100, and No. 200
designations with square openings conforming to AASHTO Designation M 92.
a. Each sieve shall be inspected visually for bent or distorted wires after each
use. Replace any damaged or nonconforming sieves.
3. Sieve shaker: Any mechanical sieve-shaking device that accomplishes the same
thoroughness of sieving as the hand-sieving procedure described in F.1.a of this
a. It is essential that the sieve shaker be designed so that its motion includes
a bumping or bouncing action sufficient to keep the aggregate particles in
motion on the surface of the sieves.
California Test 202
b. Refer to Section F.1.b of this method for procedures to verify shaker
4. Agitator (Figure 1): A mechanical device designed to hold the wash vessel in an
upright position while subjecting it to a lateral reciprocating motion at a rate of
285 ± 10 complete cycles per minute. The reciprocating motion shall be produced
by means of an eccentric located in the base of the carrier, and the length of the
stroke shall be 1.75 in. 0.025 in. The clearance between the cam and follower of
the eccentric shall be between 0.001 in. and 0.004 in. Other types of agitators may
be used provided the length of time and other factors are adjusted to produce the
same results as those obtained using the agitator described above.
5. A combination sieve shaker-agitator is allowable when it meets the above
requirements for shaking (3.a & b) while in the shaking mode and agitation (4)
while in the agitation mode. A Tyler portable sieve shaker meets the above
requirements when modified according to TL drawing No. D536.
6. Mechanical Washing Vessel: A flat-bottom, straight-sided, cylindrical vessel
conforming to the specifications and dimensions shown in Figure 2.
7. An oven or other suitable thermo-statically controlled heating device capable of
maintaining a temperature of 230˚F ± 9˚F.
Distilled, deionized, or good-quality tap water shall be used for washing the fine-aggregate test
E. SIZE OF SAMPLE
1. The sample to be tested shall be of sufficient size to ensure representation of the
material. The exact amount of material required will vary according to the nominal
size of the aggregate and the particle-size distribution.
2. Recommended sample mass for each aggregate size of processed aggregates (such
as sized aggregates for PCC and AC) or composite aggregates (such as AB and CTB)
that are comprised of approximately 40 % or more of aggregate retained on the No.
4 sieve, are listed in Table 1.
Mass of Portion
No. 4 Sieve
Over 2 ½ in. 30,000 g
2 ½ in. 25,000 g
2 in. 20,000 g
1 ½ in. 15,000 g
1 in. 10,000 g
3/4 in. 5,000 g
½ in. 2,500 g
3/8 in. 1,000 g
California Test 202
3. Sample size, for materials not adaptable to the recommendations in paragraph 2,
should be sufficient to yield the amounts noted below for each coarse-size fraction
that makes up 5 % or more of the total sample.
a. At least 1,000 g of coarse-size fractions equal to or larger than ¾ in.
b. At least 500 g of coarse-size fractions smaller than ¾ in.
4. Samples containing more than 15 % passing the No. 4 sieve shall be of sufficient
size to yield at least 1,000 g of material passing the No. 4 sieve.
F. SIEVING PROCEDURE
1. Separate the test sample into a series of sizes using such sieves as are necessary to
determine compliance with the specifications for the material being tested. Either
the hand or mechanical sieving method may be used.
a. Perform the hand method of sieving by means of a lateral and vertical
motion of the sieve, accompanied by a jarring action, so as to keep the
sample moving continuously over the surface of the sieve. Do not turn or
manipulate particles through the sieve by hand. Continue sieving until not
more than 0.5 % by mass of the total sample will pass any sieve during one
additional minute of hand sieving.
b. Mechanical sieving may be used only after it has been demonstrated that
the shaker will separate a test sample with the same effectiveness as the
hand method. The effectiveness of the mechanical shaker and the
minimum shaking time shall be determined for each shaker by comparison
with the hand-sieving method using the procedure described below.
(1) Obtain a test sample of all crushed, clean, durable aggregate with a
relatively uniform size distribution over the range of sieves to be
(2) Determine the total mass of the test sample and the tare mass of
(3) Separate the sample into its various sieve sizes using the
mechanical shaker operated for a trial period.
(4) At the end of the trial period, determine the amount of material
retained on each sieve by weighing the sieves and retained material
and subtracting the mass of the sieve.
(5) Reassemble the sieves in the mechanical shaker, and shake for an
additional period of time of not less than 1 min.
(6) Determine the amount of material on each sieve as in step (4).
(7) Repeat steps (4) through (6) until not more than 0.5 % by mass of
the total sample passes through any of the sieves during the
additional shaking time.
(8) Sieve each size fraction for one additional minute using the hand-
California Test 202
(9) If more than 0.5 % by mass of the total sample passes through any
sieve during the hand sieving, the mechanical shaker is not
performing effectively, and it shall not be used.
(10) The required shaking time for the shaker shall be at least 125 % of
the minimum time required to accomplish the thoroughness of
sieving described above. In no case shall the shaking time for any
shaker be less than 5 min.
c. When sieving, limit the amount of material retained on the No. 4 and
coarser sieves to a single layer of aggregate. If necessary, sieve the test
sample in portions; then combine all respective portions retained on the
sieves before weighing.
d. In no case, when sieving fine aggregate (material passing the No. 4 sieve),
shall the material retained on any sieve at the completion of the sieving
operation exceed that mass specified in Table 2. To reduce the amount of
material retained on a sieve, either use a sieve with openings slightly larger
than the overloaded sieve, or split the entire sample into smaller portions
prior to sieving, and then combine respective fractions prior to weighing.
MAXIMUM MASS IN GRAMS OF MATERIAL ALLOWED ON SIEVE* AT COMPLETION
OF SIEVING OPERATION
Wt. Per sq.
No. 8 4.0 200
16 3.0 150
30 2.5 125
50 2.0 100
100 1.5 75
200 1.0 50
*For intermediate sieve sizes not listed in this table, the mass specified for the next sm